In the direct bonding of orthodontic attachments to the teeth, nature of the enamel surface, the conditioning procedure, the type of adhesive and the design of the bracket base may influence the bond strength .
Ceramic orthodontic brackets were introduced in dentistry in the 1980s to satisfy the aesthetic needs of patients and have been available for clinical use since 1987 [2,3]. All currently available ceramic orthodontic brackets are composed of aluminium oxides [4,5] which have many advantages such as biocompatibility, good aesthetics, resistance to temperature and chemical changes, and good bond strength that is higher or equal to that of stainless steel brackets [6-9]. Ceramic bracket bonding mechanisms are divided into three groups: mechanically retentive bases, silane-treated chemically retentive bases, and both mechanically and chemically retentive bases. Various studies have shown that the bond strength between the ceramic and composite in a silane treated chemically retentive bracket is more as compared to a mechanically retentive ceramic bracket. This high bond strength is almost equal to the strength of enamel, making enamel fractures more likely to occur [9-15]. Therefore, mechanically retentive ceramic bracket base designs are more desirable than chemically retentive ceramic brackets .
For mechanical retention, various base designs, such as micro-crystalline, mechanical ball, dovetail, dimpled, mechanical, buttons,
and polymeric bases are available from many manufacturers. Furthermore, these designs are claimed to have more consistent bond strengths and debonding characteristics than conventional stainless steel brackets which have a mesh welded to the bracket base to provide mechanical retention [3,17,18].
Bonding can be done either by using precoated bracket system or by manually applying adhesive to the bracket base prior to placement . Precoated brackets were available as both metallic and ceramic types. Cooper RB et al., in their study claimed the advantages of adhesive precoated brackets which include consistent quality and quantity of light cure adhesives, easier clean-up following bonding, faster bonding procedure and lesser chair side time . In both systems, complete removal of flash is advocated. Leaving behind flash exposes a rough surface of composite which acts as a critical site of plaque accumulation [19,21-23]. This plaque accumulation can lead to enamel deminera-lization and white spot lesions which will compromise the final aesthetic outcome of the treatment [24,25]. The company 3M Unitek (Monrovia, California) has developed a new APC Flash-free Adhesive Coated Appliance System as an attempt to eliminate the need for flash removal. In this system optimal amount of adhesive is pre-pasted on each bracket base allowing the clinician to cure the composite without flash removal .
The aims and objectives of the present study were the following: To evaluate the effect of base designs of different ceramic brackets
Keywords:Adhesive precoated base, Fracture sites, Microcrystalline mechanical base, Polymer mesh base, Patented bead ball base
Shear Bond Strength of Ceramic
Brackets with Different Base Designs:
Comparative In-vitro Study
MohD. YounuS AnSAri1, DeepAk k AgArwAl2, Ankur guptA3, preeti BhAttAchArYA4, Juhi AnSAr5, rAvi BhAnDAri6
Introduction: Knowledge about the Shear Bond Strength (SBS)
of ceramic brackets with different base design is essential as it affects bond strength to enamel.
Aim: The aim of the present study was to evaluate and compare
the effect of base designs of different ceramic brackets on SBS, and to determine the fracture site after debonding.
Materials and Methods: Four groups of ceramic brackets
and one group of metal brackets with different base designs were used. Adhesive precoated base of Clarity Advanced (APC Flash-free) (Unitek/3M, Monrovia, California), microcrystalline base of Clarity Advanced (Unitek/3M, Monrovia, California), polymer mesh base of InVu (TP Orthodontics, Inc., La Porte, IN, United States), patented bead ball base of Inspire Ice (Ormco, Glendora, California), and a mechanical mesh base of Gemini Metal bracket (Unitek/3M, Monrovia, California). Ten brackets of each type were bonded to 50 maxillary premolars with Transbond XT (Unitek/3M). Samples were stored in distilled water at room temperature for 24 hours and subsequently tested in shear
mode on a universal testing machine (Model 3382; Instron Corp., Canton, Massachusetts, USA) at a cross head speed of 1mm/minute with the help of a chisel. The debonded interface was recorded and analyzed to determine the predominant bond failure site under an optical microscope (Stereomicroscope) at 10X magnification. One way analysis of variance (ANOVA) was used to compare SBS. Tukey’s significant differences tests were used for post-hoc comparisons. The Adhesive Remnant Index (ARI) scores were compared by chi-square test.
results: Mean SBS of microcrystalline base (27.26±1.73), was
the highest followed by bead ball base (23.45±5.09), adhesive precoated base (20.13±5.20), polymer mesh base (17.54±1.91), and mechanical mesh base (17.50±2.41) the least. Comparing the frequency (%) of ARI Score among the groups, chi-square test showed significantly different ARI scores among the groups (χ2 = 34.07, p<0.001).
conclusion: Different base designs of metal and ceramic
Keywords:Adhesive precoated base, Fracture sites, Microcrystalline mechanical base, Polymer mesh base, Patented bead ball base
group name of Bracket Manufacturer type DesignBase
Area of Base
Unitek/3M Monrovia, California
Polycrystalline Precoated Adhesive (APC)
3. InVu TP Orthodontics La Porte, IN, USA
Polycrystalline Polymer mesh 14.90
4. Inspire Ice
Ormco, Glendora California
Monocrystalline with Sapphire
Patented bead ball 11.50
[table/Fig-1]: Identification of brackets.
on SBS; comparison of the SBS among various currently available ceramic brackets, SBS between the APC Flash-Free Adhesive coated brackets and the manually pasted ceramic brackets, SBS between different ceramic brackets and mechanical mesh base metal brackets, and to determine the fracture site after debonding.
MAtErIALS And MEtHOdS
The sample comprising of 50 extracted maxillary premolars was collected from the patients who reported to the Department of Orthodontics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India, requiring orthodontic treatment. An informed and written consent from the patients and their guardians was obtained. Five groups of direct-bonded maxillary premolar brackets (4 ceramic and 1 metal) with different base designs were obtained from different manufacturers. Ten brackets were taken in each group. Identification of brackets is shown in [Table/Fig-1,2a-e]. The teeth were cleaned with tap water to remove soft tissue and debris and placed in 0.1% thymol solution (an anti-microbial solution for inhibition of bacterial growth) for one week and then stored in distilled water until use .
The criteria for tooth selection were as follows:
(1) The teeth with intact crown, unattrited and free from hypoplastic areas, cracks, gross irregularities, decays and fractures. (2) Teeth without pre-treatment with chemical agents, such as
hydrogen peroxide, formalin, or fluoride.
The samples were randomly divided into five groups (Group 1-5) each consisting of ten teeth. Each tooth was placed in a metal mold and roots were embedded in self-curing acrylic resin (width=15mm; breadth=7mm; height =18mm) upto 1mm apical to cementoenamel junction. The long axis of the tooth was kept parallel to the long axis of the metal mold. Crowns were kept
exposed to facilitate surface treatment and bracket bonding on buccal surface .
Before bonding, the facial surface of each premolar was cleaned for 10 seconds with a mixture of water and fluoride-free pumice in a rubber polishing cup using a low-speed contra-angle hand piece. The enamel surface was water rinsed to remove pumice or debris and then dried with an oil-free compressed air . Instructions of the manufacturer were carefully followed for the bonding of the bracket using light-cured orthodontic adhesive Transbond XT (Unitek/3M) consisting of an orthodontic bonding paste and an enamel bonding sealing resin. The buccal surface of the teeth was etched with 37% phosphoric acid gel, Scotchbond (3M) ESPE, for 30 seconds [30,31] followed by thorough washing and drying until a characteristic frosty white etched area was observed. A thin layer of primer (Transbond XT primer, 3M Dental Products) was applied on the etched enamel, and polymerized for five seconds. The adhesive (Transbond XT 3M Unitek) was placed on bracket base.
The bracket was placed firmly on the tooth to desired position and angulation. The excess composite resin was removed carefully from the bracket margin with a dental probe to eliminate any increase in nominal base area and were then light cured by light curing unit for ten seconds on the mesial and 10 seconds on the distal side  (total cure time is 20 seconds). All 50 teeth in each five groups with various types of brackets used the same type of bonding technique.
After bonding, all samples were stored in distilled water at room temperature for 24 hours and subsequently tested in shear mode on a universal testing machine (Model 3382; Instron Corp., Canton, Massachusetts, USA) at a cross head speed of 1mm/ minute connected to a computer that recorded the results of each test [Table/Fig-3].
The specimens were secured in the lower jaw of the machine so that the bonded brackets base was parallel to the shear force direction. Force applying chisel was secured in upper jaw and specimens were stressed in an occlusogingival direction at the bracket-tooth interface with the help of chisel [Table/Fig-4]. Upper jaw was moved at a crosshead speed of 1mm/minute , the maximum load necessary to debond or initiate bracket-tooth interface fracture was recorded in Newtons and then converted into Megapascals as a ratio of Newtons to surface area of the bracket  (SBS in MPa).
Bond strength in MPa = Force (in Newton)/Surface area of bracket (in mm2). After shear mode testing, enamel surfaces of teeth were
inspected independently by one evaluator. An optical microscope (Stereomicroscope) at 10X magnification was used to determine the Adhesive Remnant Index (ARI) score at the site of bond failure. This scale ranges from 0 to 3 .
Score 0 = no adhesive remaining on the tooth in the bonding area
Score 1 = less than half the bonded area covered by the adhesive
[table/Fig-2]: (a) Adhesive precoated base of Clarity advanced (APC Flash-free) ceramic bracket; (b) Microcrystalline base of Clarity advanced ceramic bracket; (c) Polymer mesh base of InVu ceramic bracket; (d) Patented bead ball base of Inspire Ice ceramic bracket; (e) Mechanical mesh base of Gemini metal bracket.
[table/Fig-3]: Universal testing machine with mounted specimen.
comparisons Mean Diff. Q p-value 95% ci of diff.
GROUP 1 vs.
GROUP 2 -7.13 6.23 p < 0.001***
-11.73 to -2.526 GROUP 1 vs.
GROUP 3 2.60 2.27 p > 0.05
-2.003 to 7.197 GROUP 1 vs.
GROUP 4 -3.32 2.90 p> 0.05 -7.915 to 1.285
GROUP 1 vs.
GROUP 5 2.55 2.23 p > 0.05 -2.046 to 7.154
GROUP 2 vs.
GROUP 3 9.72 8.50 p < 0.001***
5.123 to 14.32 GROUP 2 vs.
GROUP 4 3.81 3.33 p > 0.05
-0.7891 to 8.411 GROUP 2 vs.
GROUP 5 9.68 8.47 p < 0.001*** 5.080 to 14.28
GROUP 3 vs.
GROUP 4 -5.91 5.17 p < 0.01** -10.51 to -1.312
GROUP 3 vs.
GROUP 5 -0.04 0.04 p > 0.05
-4.643 to 4.557 GROUP 4 vs.
GROUP 5 5.87 5.13 p< 0.01**
1.269 to 10.47
Score 2 = more than half the bonded area covered by the adhesive
Score 3 = All adhesive remaining on the entire bonded area. SBS data were summarized as Mean±SD and compared by one way analysis of variance (ANOVA) and the significance of mean difference between the groups was done by Tukey’s post-hoc test. The ARI scores were summarized in number and percentage and compared by chi-square (χ2) test. A two-tailed p-value less than
0.05 (p<0.05) was considered statistically significant. All analyses were performed on SPSS software (windows version 17.0).
The present study determines and compares the shear bond strength of ceramic brackets with different base designs. The range mean (± SD) and median of SBS (MPa) of five groups are summarized in [Table/Fig-5].
The mean SBS of Clarity Advanced was the highest followed by Inspire Ice, Clarity Advanced (APC Flash-free), Gemini Metal and InVu the least (InVu < Gemini Metal < Clarity Advanced (APC Flash-free) < Inspire Ice < Clarity Advanced). Further, coefficient of variation (%) showed that SBS of Clarity Advanced to be least variable (6.34%) followed by InVu (10.91%), Gemini Metal (13.68%), Inspire Ice (21.72%) and Clarity Advanced (APC Flash-free) (25.80%) the highest [Table/Fig-5].
Evaluating the effect of groups on SBS, ANOVA revealed significant effect of groups on SBS (F=13.28, p<0.001) [Table/Fig-5]. Further, comparison of the mean SBS among different groups using Tukey’s test showed the following results [Table/Fig-6].
Adhesive remnant Index Score: The ARI score of five groups is summarized in [Table/Fig-7]. The frequency (%) of 0 was highest
for InVu (30%) and Gemini Metal (30%), 1 was highest for InVu (60%), 2 was highest for Clarity Advanced (APC Flash-free) (30%) and 3 was highest for Clarity Advanced (80%) [Table/Fig-7]. Chi-square (χ2) test was used to compare the frequency (%) of
ARI score among the groups. It showed significantly different ARI scores among the groups (χ2=34.07, p<0.001).
Ceramic brackets are available in many forms. The expensive ceramic brackets include monocrystalline brackets which have excellent aesthetics while the less expensive ceramic brackets are the polycrystalline brackets which have comparatively poorer aesthetics. One of the important and challenging requirements of these ceramic brackets is to be able to provide adequate bond strength during the orthodontic treatment alongwith easy debonding procedure resulting in minimal damage to the enamel surface. Since, majority of ceramic brackets depend on the mechanical retention to form an acceptable bond, the base designs play an important role in the SBS values. The advantage of the ceramic bracket over metal bracket is affinity of the ceramic brackets to incident light which allows more transmission of light onto the bracket base resulting in high polymerization of the adhesive and thus, providing a high SBS .
Several factors such as method of enamel conditioning, com-position of adhesive, bracket retention mechanism as well as method of debonding influence the forces applied for debonding the brackets. In the present study, similar debonding conditions were kept in all the five groups to minimize the variables influencing the debonding characteristics. The results indicated that different base designs have different effects on SBS. Base design charac-teristics were the reason for these results. These results were in accordance with studies conducted by Kang DY et al., and Sharma-Sayal SK et al., [16,36].
In the present study, when comparing the mean SBS of different bracket systems, it was observed that the mean SBS of microcrystalline base (Clarity Advanced) was the highest followed by bead ball base (Inspire ice), Adhesive precoated brackets (Clarity Advanced APC Flash-free), polymer mesh base (InVu), while the bracket system with the least mean SBS was of mechanical mesh base (Gemini Metal). The Clarity Advanced ceramic bracket with microcrystalline base is composed of small glass particles fused to a polycrystalline alumina, which increases the surface area available for adequate bonding and thus, the bond strength. These results were in accordance with studies conducted by Park MG and Kang DY et al., [2,16].
Result showed that the mean SBS of Clarity Advanced (APC Flash-free) was lower than that of Clarity Advanced ceramic brackets showing a significant statistical difference [Table/Fig-6]. These results were in accordance with Bearn et al., Oliver BM et al., Wong M and Power S and Cal Neto JP et al., who reported that the mean SBS of ceramic brackets which were manually coated and bonded with Transbond XT was significantly higher than the adhesive precoated brackets and also the rate of bond failure was higher with adhesive precoated brackets as compared to the conventional brackets [37-40]. Although in contrast to this study Lee M and Kanavakis G observed that the SBS of APC Flash–free
groups n Min Max Mean SD cov
Group 1 10 13.20 29.13 20.13 5.20 25.80 20.65
Group 2 10 23.25 28.89 27.26 1.73 6.34 28.04
Group 3 10 13.67 20.69 17.54 1.91 10.91 17.85
Group 4 10 14.34 31.78 23.45 5.09 21.72 23.82
Group 5 10 13.76 22.24 17.50 2.41 13.68 17.26
[table/Fig-5]: Shear bond strength of five groups.
Min: Minimum, Max: Maximum, SD: Standard deviation, COV: Coefficient of variation, F: ANOVA F value
[table/Fig-6]: Comparison of mean shear bond strength (MPa) between groups by Tukey’s test.
CI: confidence interval, p>0.05 (not significant), **p<0.01 (moderate significant), ***p<0.001 (highly significant)
group 1 (n=10) (%)
group 2 (n=10) (%)
group 3 (n=10) (%)
group 4 (n=10) (%)
group 5 (n=10) (%)
p-0 0 (0) 0 (0) 3 (30) 0 (0) 3 (30)
1 2 (20) 0 (0) 6 (60) 1 (10) 5 (50)
2 3 (30) 2 (20) 1 (10) 2 (20) 2 (20)
3 5 (50) 8 (80) 0 (0) 7 (70) 0 (0)
[table/Fig-7]: Comparison of frequency (%) of ARI scores among five groups.
group was significantly greater than the manually pasted Clarity Advanced ceramic bracket .
Also, there was statistically significant and higher SBS of Inspire Ice than InVu and Gemini Metal [Table/Fig-6]. The bead base surface of Inspire Ice has many round monocrystalline beads as completely distributed over the base surface as possible. These small beads have undercuts for mechanical interlocking of the adhesive resin resulting in the statistically higher SBS than InVu and Gemini Metal brackets. These results were in accordance with studies conducted by Park MG, Kukiattrakoon B and Samruajbenjakul B [2,3,41].
Results also showed that the mean SBS of InVu was lowest among all ceramic brackets [Table/Fig-6]. Since the InVu brackets were the largest (whole bracket base surface area) as compared with the other ceramic brackets, the greater bonding area reduced the bond strength. This is in accordance with a previous study using finite element analysis which stated that bond strength is inversely proportional to the bonding area of the bracket . The larger the bonding area, the higher is the probability that a flaw of critical size is present. Thus, a specific base design which provides a favourable stress distribution should be preferred rather than increasing the bracket dimensions. Irregular surface base of Clarity Advanced and bead ball base of Inspire Ice used in this study may decrease bracket base dimension without affecting SBS. These results were in accordance with studies conducted by Kang DY et al., .
Result also showed that the mean SBS of Gemini Metal brackets was lowest among all brackets used in the present study. The lower SBS values of stainless steel brackets are probably due to insufficient light transmission by the shadowing effect of metallic structure as also reported by Park MG and Eslamian L et al., [2,43].
When the bond is tested for failure, there are three main failure sites . These are the bracket base/adhesive interface, the enamel/adhesive interface and cohesive failure.
Highest ARI score 3 was found for Clarity Advanced (80%), Inspire Ice (70%) and Clarity Advanced (APC Flash-free) (50%). This means that debonded brackets had no adhesive remaining on the bracket base and all adhesive remaining on tooth surface resulting in a reduced enamel fracture risk and ultimate bracket bond strength. These results were in accordance with studies conducted by Kukiattrakoon B, Soderquist SA and Samruajbenjakul B et al., [3,32,41].
Lower ARI score 1 was found for InVu and Gemini Metal. This means that debonded brackets had more adhesive remaining on the bracket base and less adhesive remaining on tooth surface resulting in comparatively lower bracket bond strength [Table/ Fig-7]. These results were similar with studies conducted by Sibi AS et al., .
In the present study, the SBS of all groups exhibited higher values than the minimum orthodontic bracket bond strength as suggested by Reynolds I and therefore, could be considered sufficient for clinical application .
The present study revealed statistically valid results but a possible limitation of this study was a small sample size. Further studies using a larger sample size and more variety of base designs are recommended.
Bonding of orthodontic brackets to the tooth surface is a necessary procedure in clinical treatment. The bond strength between a bracket and the tooth surface must be highly reliable and is the key to therapeutic success. The present study determined the
effect of different bracket base designs on the SBS of orthodontic brackets bonded with Transbond XT. The debonded location of the orthodontic brackets bonded with different base designs were also studied using Stereomicroscope. It was concluded that the mean SBS of Clarity Advanced was significantly higher than Clarity Advanced (APC Flash-free) and InVu. No statistically significant difference was found on comparing Clarity Advanced with Inspire Ice and Clarity Advanced (APC Flash-free) brackets with InVu and Inspire Ice brackets. Between the ceramic brackets and mechanical mesh base metal brackets, it was found that Gemini Metal bracket showed significantly lower SBS than Clarity Advanced and Inspire Ice. However, there were no statistically significant differences when compared with Clarity Advanced (APC Flash-free) and InVu. Comparison of the ARI scores among different groups led to the conclusion that there were significantly (p<0.001) different ARI scores i.e., fracture sites were different among different brackets used.
Ferguson JW, Read MJF, Watts DC. Bond strengths of an integral bracket-base
combination: An in vitro study. Eur J Orthod. 1984;6(4):267-76.
Park MG. Effect of a DPSS laser on the shear bond strength of ceramic brackets
with different base designs. Lasers Med Sci. 2013;28:1461-66.
Kukiattrakoon B and Samruajbenjakul B. Shear bond strength of ceramic
brackets with various base designs bonded to aluminous and fluorapatite ceramics. Eur J Orthod. 2010;32:87-93.
Harris AM, Joseph VP, Rossouw PE. Shear peel bond strengths of esthetic
orthodontic brackets. Am J Orthod and Dentofac Orthop. 1992;102:215-19. Karamouzos A, Athanasiou AE, Papadopoulos MA. Clinical characteristics and
properties of ceramic brackets: A comprehensive review. Am J Orthod Dentofac
Odegaard J, Segner D. Shear bond strength of metal brackets compared with a
new ceramic bracket. Am J Orthod Dentofac Orthop. 1988;94:201-06. Swartz ML. Ceramic brackets.
 J Clin Orthod. 1988;22:82-88.
Flores DA, Caruso JM, Scott GE, Jeiroudi MT. The fracture strength of ceramic
brackets: A comparative study. Angle Orthod. 1990;60:269-76.
 Viazis AD, Cavanaugh G, Bevis RR. Bond strength of ceramic brackets under shear stress: An in vitro report. Am J Orthod Dentofac Orthop. 1990;98(3):214-21. Bordeaux JM, Moore RN, Bagby MD. Comparative evaluation of ceramic bracket
base designs. Am J Orthod Dentofac Orthop. 1994;102:552-60.
Bishara SE, Fehr DE. Ceramic brackets: Something old, something new, a review
Semin Orthod. 1997;3:178-88.
Gautam P, Valiathan A. Ceramic brackets: In search of an ideal! trends in
biomaterials and artificial organs. 2007;20:122-26.
Falkensammer F, Jonke E, Bertl M, Freudenthaler J, Bantleon HP. Rebonding
performance of different ceramic brackets conditioned with a new silane coupling agent. Eur J Orthod. 2013;35(1):103-09.
Gittner R, Muller-Hartwich R, Engel S, Jost-Brinkmann PG. Shear bond
strength and enamel fracture behavior of ceramic brackets Fascination® and Fascination®2. J Orofac Orthop. 2012;73:49-57.
Eliades T, Viazis AD, Lekka M. Failure mode analysis of ceramic brackets bonded
to enamel. Am J Orthod Dentofac Orthop. 1993;104:21-26.
Kang DY, Choi SH. Quantitative analysis of mechanically retentive ceramic
bracket base surfaces with a three-dimensional imaging system. Angle Orthod. 2013;83:705-711.
Russell JS. Aesthetic orthodontic brackets.
 J Orthod. 2005;32:146-63.
Matasa CG. Direct bonding metallic brackets: Where are they heading?
 Am J
Orthod Dentofac Orthop. 1992;101:552-60.
Armstrong D, Shen G, Petocz P, Darendeliler MA. Excess adhesive flash upon
bracket placement. Angle Orthod. 2007;77:1101-08.
Cooper RB, Goss M, Hamulla W. Direct bonding with light cured adhesive
precoated brackets. J Clin Orthod. 1992;26(8):477-79.
Sukontapatipark W, El-Agroudi MA, Selliseth NJ, Thunold K, Selvig KA. Bacterial
colonization associated with fixed orthodontic appliances: A scanning electron microscopy study. Eur J Orthod. 2001;23:475-84.
Gwinnett AJ, Ceen RF. Plaque distribution on bonded brackets: A scanning
microscope study. Am J Orthod Dentofac Orthop. 1979;75:667-77.
Weitman RT, Eames WB. Plaque accumulation on composite surfaces after
various finishing procedures. J Am Dent Assoc. 1975;91:101-06.
Ogaard B, Rella G, Arends J. Orthodontic appliances and enamel demineralization.
Part 1. Lesion development. Am J Orthod Dentofac Orthop. 1988;94:68-73. Maxfield BJ, Hamdan AM, Tufekc IE, Shroff B, Best AM, Lindauer SJ.
Development of white spot lesions during orthodontic treatment: Perceptions of patients, parents, orthodontists, and general dentists. Am J Orthod Dentofac
Lee M, Kanavakis G. Comparision of shear bond strength and bonding time of
novel flash-free bonding system. Angle Orthod. 2016;86(2):265-70.
Katona TR, Long RW. Effect of loading mode on bond strength of orthodontic
Bishara SE, VonWald L, Laffoon JF, Warren JJ. Effect of a self-etch primer/
adhesive on the shear bond strength of orthodontic brackets. Am J Orthod
Dentofac Orthop. 2001;119:621-24.
Wang WN, Meng CL, Tarng TH, Bond strength: A comparison between chemical
coated and mechanical interlock bases of ceramic and metal brackets. Am J
Orthod Dentofac Orthop. 1997;111(4);374-81.
Gardner A, Hobson R. Variations in acid-etch patterns with different acids and
etch times. Am J Orthod Dentofac Orthop. 2001;120(1):64-67.
Shannon M. Bond strength of orthodontic brackets with varying etch duration.
Clin Orthod. 1982:130-32.
Soderquist SA, Drummond JL, Evans CA. Bond strength evaluation of ceramic
and stainless steel bracket bases subjected to cyclic tensile loading. Am J
Orthod Dentofac Orthop. 2006;129(2):175.e7-e12.
Cacciafesta V, Sfondrini MF, Angelis MD, Scribante A, Klersy C. Effect of water
and saliva contamination on shear bond strength of brackets bonded with conventional, hydrophilic, and self-etching primers. Am J Orthod Dentofac
Fox NA, McCabe JF, Buckley JG. A critique of bond strength testing in
orthodontics. Br J Orthod. 1994;2:33-43.
Maijer R, Smith DC. Variables influencing the bond strength of metal orthodontic
bracket bases. Am J Orthod Dentofac Orthop.1981;79: 20-34.
Sharma-Sayal SK, Rossouw PE, Kulkarni GV, Titley KC. The influence of
orthodontic bracket base design on shear bond strength. Am J Orthod Dentofac
Bearn, Aird JC, McCabe JF. Ex vivo bond strength of adhesive precoated metallic
and ceramic brackets. Br J Orthod. 1995;22:233-36.
Oliver BM, Dama M, Normandin G. Rate of bond failure of adhesive precoated
brackects: A clinical survey. Orthod Cyber J. 1996;1:3.
Wong M, Power S. A prospective randomized clinical trial to compare precoated
and nonprecoated brackets. J Orthod. 2003; 30:155-58.
Cal-Neto JP, Miguel JA, Zanella E. Effect of a self-etching primer on shear bond
strength of adhesive precoated brackets in vivo. Angle Orthod. 2006;76:127-31.
Samruajbenjakul B, Kukiattrakoon B. Shear bond strength of ceramic brackets
with different base designs to feldspathic porcelains. Angle Orthod. 2009;79: 571–76.
Lopez JI. Retentive shear strengths of various bonding attachments bases.
J Orthod Dentofac Orthop.1980;77: 669-78.
Eslamian L, Borzabadi-Farahani A, Mousavi N, Ghasemi A. A comparative study
of shear bond strength between metal and ceramic brackets and artificially aged composite restorations using different surface treatments. Eur J Orthod. 2012; 34:610–17.
O’Brien KD, Watts DC, Read MJF. Residual debris and bond strength- Is there a
relationship? Am J Orthod Dentofac Orthop. 1988;94:222-30.
Sibi AS, Kumar S, Sundareswaran S, Philip K, Pillai B. An in vitro evaluation of
shear bond strength of adhesive precoated brackets. J Ind Orthod Soc. 2014; 48(2):97-103.
 Reynolds I. A review of direct orthodontic bonding. Br J Orthod. 1975;2:171-78.
pArticulArS oF contriButorS:
1. Postgraduate Student, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India. 2. Professor and HOD, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India. 3. Reader, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India.
4. Professor, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India. 5. Senior Lecturer, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India. 6. Senior Lecturer, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly, Uttar Pradesh, India.
nAMe, ADDreSS, e-MAil iD oF the correSponDing Author: Dr. Ankur Gupta,
Reader, Department of Orthodontics and Dentofacial Orthopedics, Institute of Dental Sciences, Bareilly– 243006, Uttar Pradesh, India.
FinAnciAl or other coMpeting intereStS: None.